Textile-type triboelectric nanogenerator using Teflon wrapping wires as wearable power source
Micro and Nano Systems Letters volume 10, Article number: 8 (2022)
Wearable electronic devices such as mobile communication devices, portable computers, and various sensors are the latest significant innovations in technology which use the Internet of Things (IoT) to track personal data. Wearable energy harvesters are required to supply electricity to such devices for the convenience of users. In this study, a textile-type triboelectric nanogenerator (T-TENG), produced using commercial electrode fibers, was fabricated to generate electrical energy using external mechanical stimulation. The commercial fiber was an electrode coated with Teflon on a copper wire with a diameter of ~ 320 μm. Using this commercial fiber, a T-TENG was easily fabricated by knitting and weaving. The performance of the T-TENG was analyzed to understand the effect of force and frequency. It was observed that the performance of the T-TENG did not degrade even under harsh conditions and treatment. The textile-type TENG possessed an energy harvesting capability with an output power density of ~ 0.36 W/m2 and could operate electronic devices by charging a capacitor.
Wearable technologies, also called “wearables”, such as mobile communication devices, portable computers, and wearable sensors using smart Internet of Things (IoT) technology have received considerable attention recently [1,2,3,4]. Wearable electronic devices require a flexible and wearable electricity supply source instead of the existing rigid solid-state electricity supply sources [5,6,7]. Therefore, research on power storage such as wearable supercapacitors and batteries are being conducted. However, even with power storage capability, external power is required for charging. Several studies have been conducted on wearable energy harvesters for supplying electricity from natural movements [8, 9] to make wearables more convenient for use. Among them, triboelectric nanogenerator (TENG) and piezoelectric nanogenerator (PENG), which produce electrical energy from external mechanical stimulation, are receiving considerable attention . However, PENGs have limitations because of their complicated manufacturing process and relatively low output power. Many studies are being conducted on TENGs that are easy to manufacture and have a low frequency and high output voltage [11, 12].
Substantial research has been conducted to produce wearable TENGs from wearable textiles [13,14,15]. The textile-type TENGs (T-TENG) are largely divided, based on the manufacturing method [16, 17], into fabric and fiber. For fabric TENGs, the fabric itself is used as a tribo-material, or the fabric is directly coated with a functional material to be used as a functional fabric [18,19,20,21]. For example, the fabric is coated with carbon nanotubes, metal nanowires, and metals (i.e., Ag, nickel, etc.) to achieve conductivity; or the fabric is coated with nylon, polydimethylsiloxane, polyurethane, etc. to make a tribo-material. The fabric-type TENG manufactured in this manner has a relatively high output power because it has a higher areal density than the fiber type, however it is limited because of its airtight properties and low durability [22, 23]. Accordingly, research is being conducted on a new T-TENG manufactured using a fiber composed of a core–shell structure [24,25,26]. A fiber is manufactured using a conductive material (carbon nanotube, liquid metal, etc.) as the core, and the tribo-material is coated with a shell around the core. The fiber can be sewed, knitted, or woven into a textile that is used for energy harvesting. However, it is difficult to use in the clothing industry because thick fibers are formed in the coating of the shell with a tribo-material, and the process of manufacturing the fibers is relatively complicated . To overcome the limitations of the existing fiber-type TENG, the easy-to-use fiber must have a thin diameter for use in the clothing industry . In addition, TENG made of these fibers must be flexible, bendable, and be capable of large-scale fabricating.
In this study, a T-TENG was fabricated to produce electrical energy using external mechanical stimulation using a commercial fiber. The commercial fiber was an electrode (copper wire with a diameter of ~ 320 μm) coated with Teflon. A large area T-TENG can be woven or knit using this fiber. The fabricated TENG is flexible and bendable; therefore, it is suitable for wearables; it is easy to connect the copper electrode inside the fiber to electronic devices. The T-TENG has an energy harvesting capability that not only has an output power density of ~ 0.36 W/m2, but also can operate electronic devices by charging a capacitor. In addition, it has good harvesting ability without degradation, even after immersion in acidic and basic solutions, owing to the hydrophobicity of Teflon. We believe that new research on energy harvesting using commercial fibers will not only be applicable to the clothing industry, but will be a new step in easily usable TENG.
Materials and methods
Yellow and blue Teflon wrapping wires (SME) were purchased from commercial vendor. A latex glove (Microflex) was purchased from commercial vendor. Special-grade hydrochloric acid (HCl, 35–37%), and electronic-grade sodium hydroxide (NaOH, 99.9%) were purchased from a commercial vendor (SAMCHUN Chemicals).
Fabrication of the textile-type triboelectric nanogenerator
The purchased Teflon wrapping wire was used without any further treatment. T-TENGs are fabricated using knitting or home weaving machines. In the case of weaving, a general yarn was used for the wrap, and Teflon wrapping wire was used for the weft. For knitting, the pattern density is controlled by adjusting the loop length of T-TENG. In this study, a knitted T-TENG was used for performance evaluation. The knitted T-TENG was fabricated with a middle pattern density and an area of 25 cm2 was fabricated for characterizing of T-TENG. The latex was used as the opposite material of Teflon for T-TENG power generation.
Scanning electron microscopy-energy dispersive X-ray spectroscopy (SEM–EDS, SU6600, Hitachi) was used to characterize the surface morphology and properties. A solenoid motor (JF-1040) was used to provide mechanical stimulation for evaluating the performance of the T-TENG. The applied force was measured by using a load cell (BONGSHIN, DBBP-20). The output voltage and current signals of the textile-type TENG were measured using an electrometer (Keithley 2400). The data collection and preprocessing system used LabVIEW software and NI collection cards that allow real-time data collection. All tests were conducted by selecting an appropriate resistance to measure the output voltage within the measurement range of the equipment.
Results and discussion
A fiber made of commercially available wire wrapped by Teflon was used to fabricate the T-TENG used for energy harvesting. The fiber was a Teflon wrapped 160 μm copper wire with a diameter of 320 μm (Fig. 1a). Figure 1b, shows that the surface was generally flat, and fluorine and carbon were common. Traditional methods such as knitting can be used with these thin and flexible wires to fabricate T-TENG (Fig. 1c). As the T-TENGs can withstands bending, wrinkling, and torsion; they can easily be converted to wearable devices (Fig. 1d). The fabricated T-TENG was characterized using a pushing machine composed of a solenoid motor and load cell that measured its force (Fig. 1e). The working principle of the fabricated T-TENG is the coupling of the triboelectrification and electrostatic induction effects. As shown in Fig. 1f, when the two materials come into contact some electrical charge is transferred from one material to the other. One material becomes negatively charged as it gains electrons; the other material loses electrons, and becomes positively charged. When the charged materials are separated, current flows in the circuit. When the two materials come close again current flows in the circuit in the opposite direction. We used Teflon, which can easily absorb electrons as one material; we used Latex as the other material because it can be positively charged as it easily loses electrons. The performance of the T-TENG was evaluated using these materials.
Many factors affect the output of the T-TENG; among them, we investigated the effect of frequency and force. The frequency and force were adjusted using a solenoid motor and LabVIEW, respectively. The resulting force was measured using a load cell under the T-TENG. First, the open-circuit voltage and closed-circuit current of the T-TENG at 1 Hz were measured according to the applied force (Fig. 2a, b). As the force increased from 5 to 40 N, the voltage output of the T-TENG increased from ~ 100 V to ~ 250 V. This increase in voltage is due to the higher force applied to the T-TENG, tighter contact between the two friction materials, and an increase in the contact area. The current output increased up to a force of 20 N and then stabilized. The output current was stabilized compared with output voltage depending on the force because the short-circuit current is proportional to the speed of contact-separation.
The output voltage and current of the T-TENG were measured while increasing the frequency from 1 to 4 Hz (Fig. 2c, d). It was established that the output voltage increased to 3 Hz and then stabilized; the output current increased as the frequency increased. The increase in the electrical output of the T-TENG with increasing frequency is attributed to the contribution of the charge transfer and charge density. The output voltage and current of the T-TENG were measured varying the resistance from 106 to 1010 Ω (Fig. 2e). As the external resistance increased, the output voltage of the T-TENG increased and the output current decreased. The power density of T-TENG was ~ 0.36 W/m2 with an external load resistance of 109 Ω (Fig. 2f). The fabricated T-TENG has a higher maximum output voltage and maximum power density compared with the previous fiber type T-TENG (Table 1).
The durability of T-TENGs in harsh environments is important for their application in wearable devices. Therefore, the ability of the T-TENG to generate electricity was tested after immersing it in 1 M acid and 1 M base for 1 h, respectively. Owing to the water repellency and chemical resistance of Teflon, there was little change in the surface after immersion compared to that before immersion (Fig. 3a, b). In addition, there was little change in performance when a pushing machine (at 1 Hz and 15 N) was used with the T-TENG (Fig. 3c). The pattern density varies by controlling the loop length of the T-TENG during knitting. The performance of the fabricated T-TENG varied depending on the pattern density, which was determined as low, middle, and high. The voltage produced increases from ~ 1 to ~ 2 V/cm2 as the pattern density increases (Fig. 3d). This is because the area where the Teflon and latex meet in the same area increases.
For practical use, the durability of the manufactured T-TENG is important. Thus, the performance of T-TENG in repeated external stimuli was tested. The relative output voltage (V/VF) did not change significantly when the contact-separation was cycled 2500 times using a pushing machine, which implies the output voltage of T-TENG was constant during the cycles (Fig. 3e). The performance of T-TENG were measured according to the cycle of bending, (Curvature: 0.35 cm−1), wrinkling, and torsion (torsion angle: 15°). In the wrinkling test, T-TENG was attached to the palm of the hand. The clenching and opening of the fist was defined as one cycle. The performance degradation of the T-TENG was negligible in the cycles of bending, wrinkling, and torsion compared with the first output voltage (Fig. 3f).
Normally, the T-TENG generates an alternating current (AC); therefore, the output must be converted to DC to power an external electronic device. A commercial capacitor was charged by connecting a rectifier circuit to the T-TENG (Fig. 4a). The capacitor was charged over 2 V while repeatedly applying contact separation with a force of 15 N at 2 Hz using a pushing machine on the T-TENG (Fig. 4b). By connecting a 4.7 μF capacitor charged over 2 V with the T-TENG to the calculator, the calculator was able to perform simple additions and multiplications for ~ 8 s (Fig. 4c). The developed T-TENG can supply power to electronic devices by harvesting mechanical energy generated by normal human motion. We fabricated an insole in a shoe (Fig. 5a) with an integrated T-TENG (area: 30 cm2). Based on the human motion of standing, walking, running, and falling, the contact separation between the socks and T-TENG is repeated to harvest energy. The output voltage varied depending on the human motion. The output voltage is higher when running than when walking (Fig. 5b). This is because the contact area between the socks and T-TENG increases during running. This indicates that the T-TENG fabricated by knitting can be used as a wearable energy source powered by human movement. In addition, there is little change in the output voltage in standing state. However, only negative output voltage occurs in the falling state (Fig. 5b). This makes it possible to distinguish a human motion state.
In this study, a T-TENG that can generate electric power via external mechanical stimulation was fabricated by knitting a commercial electrode as a fiber. The output voltage and current were measured according to the applied frequency and magnitude of the force, and the output power density was measured according to the resistance. The fabricated T-TENG had an output power density of ~ 0.36 W/m2. We confirmed that it worked satisfactorily without degradation even in harsh external conditions. In addition, the T-TENG could charge a capacitor to drive electronic devices. We believe that, in the future, the fabricated T-TENGs could be used in wearable electronics with working environments such as bending and twisting.
Availability of data and materials
All data generated or analysed during this study are included in this published article.
Internet of Things
Textile-type triboelectric nanogenerator
Mamdiwar SD, Shakruwala Z, Chadha U, Srinivasan K, Chang C-Y (2021) Recent advances on IoT-assisted wearable sensor systems for healthcare monitoring. Biosensors 11(10):372. https://doi.org/10.3390/bios11100372
Mayer M, Baeumner AJ (2019) A megatrend challenging analytical chemistry: biosensor and chemosensor concepts ready for the internet of things. Chem Rev 119(13):7996–8027. https://doi.org/10.1021/acs.chemrev.8b00719
Lou Z, Wang L, Shen G (2018) Recent advances in smart wearable sensing systems. AdvMater Technol 3(12):1800444. https://doi.org/10.1002/admt.201800444
Chen G, Xiao X, Zhao X, Tat T, Bick M, Chen J (2021) Electronic textiles for wearable point-of-care systems. Chem Rev 122(3):3259–3291. https://doi.org/10.1021/acs.chemrev.1c00502
Xu C, Song Y, Han M, Zhang H (2021) Portable and wearable self-powered systems based on emerging energy harvesting technology. Microsyst Nanoeng 7(1):1–14. https://doi.org/10.1038/s41378-021-00248-z
Macário D, Domingos I, Carvalho N, Pinho P, Alves H (2022) Harvesting circuits for triboelectric nanogenerators for wearable applications. iScience 25(4):103977. https://doi.org/10.1016/j.isci.2022.103977
Zhang S, Xia Q, Ma S, Yang W, Wang Q, Yang C, Jin B, Liu C (2021) Current advances and challenges in nanosheet-based wearable power supply devices. iScience 24(12):103477. https://doi.org/10.1016/j.isci.2021.103477
Zou Y, Raveendran V, Chen J (2020) Wearable triboelectric nanogenerators for biomechanical energy harvesting. Nano Energy 77:105303. https://doi.org/10.1016/j.nanoen.2020.105303
Shi Q, Dong B, He T, Sun Z, Zhu J, Zhang Z, Lee C (2020) Progress in wearable electronics/photonics—moving toward the era of artificial intelligence and internet of things. InfoMat 2(6):1131–1162. https://doi.org/10.1002/inf2.12122
Haroun AF, Le X, Gao S, Dong B, He T, Zhang Z, Wen F, Xu S, Lee C (2021) Progress in micro/nano sensors and nanoenergy for future AIoT-based smart home applications. Nano Express 2:022005. https://doi.org/10.1088/2632-959X/abf3d4
Zhu G, Peng B, Chen J, Jing Q, Wang ZL (2015) Triboelectric nanogenerators as a new energy technology: from fundamentals, devices, to applications. Nano Energy 14:126–138. https://doi.org/10.1016/j.nanoen.2014.11.050
Tan P, Zheng Q, Zou Y, Shi B, Jiang D, Qu X, Ouyang H, Zhao C, Cao Y, Fan Y (2019) A battery-like self-charge universal module for motional energy harvest. Adv Energy Mater 9(36):1901875. https://doi.org/10.1002/aenm.201901875
Lee S, Ko W, Oh Y, Lee J, Baek G, Lee Y, Sohn J, Cha S, Kim J, Park J, Hong J (2015) Triboelectric energy harvester based on wearable textile platforms employing various surface morphologies. Nano Energy 12:410–418. https://doi.org/10.1016/j.nanoen.2015.01.009
Rana SMS, Zahed MA, Rahman MT, Salauddin M, Lee SH, Park C, Maharjan P, Bhatta T, Shrestha K, Park JY (2021) Cobalt-Nanoporous carbon functionalized nanocomposite-based triboelectric nanogenerator for contactless and sustainable self-powered sensor systems. Adv Funct Mater 31(52):2105110. https://doi.org/10.1002/adfm.202105110
Sahu M, Hajra S, Panda S, Rajaitha M, Panigrahi BK, Rubahn H-G, Mishra YK, Kim HJ (2022) Waste textiles as the versatile triboelectric energy-harvesting platform for self-powered applications in sports and athletics. Nano Energy 97:107208. https://doi.org/10.1016/j.nanoen.2022.107208
Huang P, Wen D-L, Qiu Y, Yang M-H, Tu C, Zhong H-S, Zhang X-S (2021) Textile-based triboelectric nanogenerators for wearable self-powered microsystems. Micromachines 12(2):158. https://doi.org/10.3390/mi12020158
Hu Y, Zheng Z (2019) Progress in textile-based triboelectric nanogenerators for smart fabrics. Nano Energy 56:16–24. https://doi.org/10.1016/j.nanoen.2018.11.025
Paosangthong W, Wagih M, Torah R, Beeby S (2019) Textile-based triboelectric nanogenerator with alternating positive and negative freestanding grating structure. Nano Energy 66:104148. https://doi.org/10.1016/j.nanoen.2019.104148
Qiu Y, Yang D, Li B, Shao S, Hu L (2018) Wearable triboelectric nanogenerators based on hybridized triboelectric modes for harvesting mechanical energy. RSC Adv 8(46):26243–26250. https://doi.org/10.1039/C8RA03677B
Liu J, Gu L, Cui N, Xu Q, Qin Y, Yang R (2019) Fabric-based triboelectric nanogenerators. Research 2019:1091632. https://doi.org/10.34133/2019/1091632
Salauddin M, Rana SMS, Rahman MT, Sharifuzzaman M, Maharjan P, Bhatta T, ChoH LSH, Park C, Shrestha K, Sharma S, Park JY (2022) Fabric-Assisted MXene/silicone nanocomposite-based triboelectric nanogenerators for self-powered sensors and wearable electronics. Adv Funct Mater 32(5):2107143. https://doi.org/10.1002/adfm.202107143
Wang J, He J, Ma L, Yao Y, Zhu X, Peng L, Liu X, Li K, Qu M (2021) A humidity-resistant, stretchable and wearable textile-based triboelectric nanogenerator for mechanical energy harvesting and multifunctional self-powered haptic sensing. Chem Eng J 423:130200. https://doi.org/10.1016/j.cej.2021.130200
Salauddin M, Rana SMS, Sharifuzzaman M, Rahman MT, Park C, Cho H, Maharjan P, Bhatta T, Park JY (2021) A Novel MXene/Ecoflex nanocomposite-coated fabric as a highly negative and stable friction layer for high-output triboelectric nanogenerators. Adv Energy Mater 11(1):2002832. https://doi.org/10.1002/aenm.202002832
Dong K, Deng J, Ding W, Wang AC, Wang P, Cheng C, Wang YC, Jin L, Gu B, Sun B (2018) Versatile core–sheath yarn for sustainable biomechanical energy harvesting and real-time human-interactive sensing. Adv Energy Mater 8(23):1801114. https://doi.org/10.1002/aenm.201801114
Lin M-F, Xiong J, Wang J, Parida K, Lee PS (2018) Core-shell nanofiber mats for tactile pressure sensor and nanogenerator applications. Nano Energy 44:248–255. https://doi.org/10.1016/j.nanoen.2017.12.004
Zheng L, Zhu M, Wu B, Li Z, Sun S, Wu P (2021) Conductance-stable liquid metal sheath-core microfibers for stretchy smart fabrics and self-powered sensing. Sci Adv 7(22):eabg4041. https://doi.org/10.1126/sciadv.abg4041
Paosangthong W, Torah R, Beeby S (2019) Recent progress on textile-based triboelectric nanogenerators. Nano Energy 55:401–423. https://doi.org/10.1016/j.nanoen.2018.10.036
Kwak SS, Yoon H-J, Kim S-W (2019) Textile-based triboelectric nanogenerators for self-powered wearable electronics. Adv Funct Mater 29(2):1804533. https://doi.org/10.1002/adfm.201804533
Dong K, Wang Y-C, Deng J, Dai Y, Zhang SL, Zou H, Gu B, Sun B, Wang ZL (2017) A highly stretchable and washable all-yarn-based self-charging knitting power textile composed of fiber triboelectric nanogenerators and supercapacitors. ACS Nano 11(9):9490–9499. https://doi.org/10.1021/acsnano.7b05317
Tong Y, Feng Z, Kim J, Robertson JL, Jia X, Johnson BN (2020) 3D printed stretchable triboelectric nanogenerator fibers and devices. Nano Energy 75:104973. https://doi.org/10.1016/j.nanoen.2020.104973
Li H, Zhao S, Du X, Wang J, Cao R, Xing Y, Li C (2018) A Compound yarn based wearable triboelectric nanogenerator for self-powered wearable electronics. Adv Mater Technol 3(6):1800065. https://doi.org/10.1002/admt.201800065
Wang W, Yu A, Liu X, Liu Y, Zhang Y, Zhu Y, Lei Y, Jia M, Zhai J, Wang ZL (2020) Large-scale fabrication of robust textile triboelectric nanogenerators. Nano Energy 71:104605. https://doi.org/10.1016/j.nanoen.2020.104605
Ren X, Xiang X, Yin H, Tang Y, Yuan H (2021) All-yarn triboelectric nanogenerator and supercapacitor based self-charging power cloth for wearable applications. Nanotechnology 32(31):315404. https://doi.org/10.1088/1361-6528/abfcfe
Pu X, Li L, Song H, Du C, Zhao Z, Jiang C, Cao G, Hu W, Wang ZL (2015) A self-charging power unit by integration of a textile triboelectric nanogenerator and a flexible lithium-ion battery for wearable electronics. Adv Mater 27(15):2472–2478. https://doi.org/10.1002/adma.201500311
Zhao Z, Yan C, Liu Z, Fu X, Peng LM, Hu Y, Zheng Z (2016) Machine-washable textile triboelectric nanogenerators for effective human respiratory monitoring through loom weaving of metallic yarns. Adv Mater 28(46):10267–10274. https://doi.org/10.1002/adma.201603679
Rezaei J, Nikfarjam A (2021) Rib stitch knitted extremely stretchable and washable textile triboelectric nanogenerator. Adv Mater Technol 6(4):2000983. https://doi.org/10.1002/admt.202000983
Gong W, Hou C, Guo Y, Zhou J, Mu J, Li Y, Zhang Q, Wang H (2017) A wearable, fibroid, self-powered active kinematic sensor based on stretchable sheath-core structural triboelectric fibers. Nano Energy 39:673–683. https://doi.org/10.1016/j.nanoen.2017.08.003
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Kim, S., Cho, W., Won, DJ. et al. Textile-type triboelectric nanogenerator using Teflon wrapping wires as wearable power source. Micro and Nano Syst Lett 10, 8 (2022). https://doi.org/10.1186/s40486-022-00150-x